- Ziegler-Natta catalyst
A Ziegler-Natta catalyst is a
reagentor a mixture of reagents used in the production of polymersof 1-alkenes (α-olefins). Ziegler-Natta catalysts are typically based on titanium compounds and organometallic aluminium compounds, for example triethylaluminium, (C2H5)3Al.
Ziegler-Natta catalysts are used to polymerize terminal 1-
alkenes.:n CH2=CHR → - [CH2-CHR] n-
Karl Ziegler, for his discovery of these titanium based catalysts, and Italian Giulio Natta, for using them to prepare stereoregular polymers, were awarded the Nobel Prize in Chemistry in 1963.
tereochemistry of poly-1-alkenes
Karl Ziegler prepared linear
polyethylenewith the catalyst he discovered. Giulio Natta used similar catalysts to polymerize 1-alkenes. Poly(1-alkene)s can be isotactic, syndiotactic, or atactic, depending on the relative orientation of the alkylgroups in polymer chains consisting of units - [CH2-CHR] -. In isotactic polymers, all chiral centers CHR share the same stereochemistry. Chiral centers in syndiotactic polymers alternate their relative stereochemistry. Atactic polymers lack regular stereochemistry. The stereoregularity of the polymer depends on the type of catalyst used to prepare it, and once prepared, the polymer's stereochemistry does not change.
The Ziegler-Natta catalysts represented a major breakthrough in polymerization chemistry because they produce a variety of commercially important polymers and can be highly stereoselective. Previously known radical polymerization reactions result in the formation of atactic polymers. TiCl4-derived catalyst systems [Hill, A.F. "Organotransition Metal Chemistry" Wiley-InterScience: New York, 2002: pp. 136-139.] , [Kissin, Y.V. "Alkene Polymerization Reactions with Transition Metal Catalysts" Elsevier: Amsterdam, 2008; Chapter 4.] , convert
propylene, and many other 1-alkenes, to isotactic polymers such as polypropylene. Related systems employing VCl4 yield syndiotactic polymers.
Preparation of the catalysts
The first Ziegler-Natta catalyst was produced by treating crystalline α-TiCl3 with [AlCl(C2H5)2] 2. Polymerization reactions of any alkene occur at special Ti centers located on the exterior of the crystallites. Most titanium ions in these crystallites are surrounded by six chloride ligands to give an
octahedralstructure. At the surface, however, "defects" occur where some Ti centers lack their full complement of chloride ligands. The alkene molecule binds at these "vacancies" . In ways that are still not fully clear, the alkene converts to an alkyl ligand group. The most probable pathway of this reaction is the insertion of the C=C bond of the alkene molecule into the Ti-C bond:
LnTi-CH2-CHR-Polymer + CH2=CHR → LnTi-CH2-CHR-CH2-CHR-Polymer
coordination sphereof the Ti atom restricts the approach of incoming alkene molecules, thereby imposing stereoregularityon the growing polymer chain.4 The Cossee-Arlman mechanismdescribes the growth of stereospecific polymers.Elschenbroich, C.; Salzer, A.; "Organometallics: a concise Introduction" VCH Verlagsgesellschaft mbH, New York, 1992, p. 423-425.] .
Many thousands of alkene insertion reactions occur at each active center resulting in the formation of long polymer chains attached to the center. On occasion, the polymer chains are disengaged from the active centers in the reaction:
LnTi-CH2-CHR-Polymer + CH2=CHR → LnTi-CH2-CH2R + CH2=CR-Polymer
This reaction occurs quite rarely and the formed polymers have a too high molecular weight to be of commercial use. To reduce the molecular weight, hydrogen is added to the polymerization reaction:
LnTi-CH2-CHR-Polymer + H2 → LnTi-H + CH3-CHR-Polymer
During the past 40 years, a large number of different supported Ziegler-Natta catalysts were developed which afford a much higher activity in alkene polymerization reactions and much higher contents of crystalline isotactic fractions in the polymers they produce, up to 97-99%. The principal source of Ti in all these catalysts is TiCl4, and the principal support is MgCl2. In order to maintain the high selectivity for an isotactic polymer product, a variety of catalyst modifiers,
Lewis bases, must be used. To form these catalysts, several techniques were developed for combining TiCl4, MgCl2, and the Lewis base in a single solid pre-catalyst. The final catalyst system is prepared by combining this solid powder with AlEt3 and another Lewis base compound.
It should be noted that titanium(IV) chloride, all solid Ziegler-Natta catalysts and alkyl aluminium compounds are unstable in air, and the alkylaluminium compounds are
pyrophoric. The catalysts, therefore, must be prepared and handled under an inert atmosphere.
Mechanism and the origin of stereospecificity
stereoregularityis believed to follow from a polymer growth mechanism known as the Cossee-Arlman mechanism, in which the polymer grows at vacant Cl sites at the Ti surface.
In the search for a deeper understanding and control of Ziegler-Natta
polymerisationat the molecular level, a number of metallocenecatalysts have been developed, often offering fine control over the composition and tacticityof the polymer chain so produced. Other organometallic compounds that are capable of forming the same stereoregular polymers as the Ziegler-Natta TiCl4 systems are metallocene compounds. One such compound is (Cp)2TiCl2; this compound does not have a vacant site like the TiCl3 crystal, and as a result, must also be activated by an alkyl aluminium compound. Most commonly the polymer MAO or methylaluminoxane ( [CH3AlO] n) is used as a cocatalyst. Like AlEt3, it activates the transition metal complex by behaving as a Lewis Acidand abstracting one of the halides to create a vacancy where the alkene can be introduced to the complex. [Bochmann, M. "Organometallics 1, Complexes with Transition Metal-Carbon σ-Bonds" Oxford University Press, New York, 1994: pp. 69-71.]
Activity and chain termination
Activity depends on the nature of the metal. Ti, Zr, and Hf form highly active catalysts.Bochmann, M. "Organometallics 2, Complexes with Transition Metal-Carbon π-Bonds" Oxford University Press, New York, 1994: pp. 57-58.] It is theorized that these catalysts feature d0 species. Without any d-electrons, the titanium-alkene bond is not stabilized by
pi backbonding, so the barrier for alkene binding is decreased.
The length of a polymer chain is determined by two competing rate constants, the rate of chain propagation (transferring the alkene to the growing polymer chain) versus the rate of termination. Termination usually occurs by β-H elimination. By tuning, one can effectively "dial in" the molecular weight of the polymer product.cite journal | author = H. G. Alt and A. Koppl | title = Effect of the Nature of Metallocene Complexes of Group IV Metals on Their Performance in Catalytic Ethylene and Propylene Polymerization | year = 2000 | journal =
Chem. Rev.| volume = 100 | issue = 4 | pages = 1205–1222 | doi=10.1021/cr9804700] For example, "half-sandwich" zirconium species, tend to give low molecular weight polymers because of their enhanced tendency to undergo β-hydride elimination.
Homogeneous Ziegler-Natta catalysts
Significant effort has been dedicated to developing other catalysts that effectively polymerize a number of branched alkenes. In addition, there has been an interest in developing homogeneous Ziegler-Natta catalysts (that don't require the aluminium cocatalyst); these species are cationic and become active in solution by losing a labile ligand. One such catalyst is the
agostic complex[Cp2Zr(CH3)CH3B(C6F5)3] . [Fink, G.; Brintzinger, H.H.; "Ziegler Catalysts" Springer-Verlag, 1995, p. 161-164.] The borate anion dissociates, leaving a vacant active site to bind alkene, allowing polymerization to commence. Developments have built upon advances in non-coordinating anions. In addition to those based on cyclopentadienylligands, catalysts are increasingly designed using nitrogen-based ligands.9
Polymers prepared by Ziegler-Natta catalysts
*Amorphous Poly-alpha-olefins (
* Takahashi, T. "Titanium(IV) Chloride-Triethylaluminum": "Encyclopedia of Reagents for Organic Synthesis." John Wiley & Sons, Ltd, 2001.
Wikimedia Foundation. 2010.
Look at other dictionaries:
Ziegler–Natta catalyst — A Ziegler–Natta catalyst is a catalyst used in the synthesis of polymers of 1 alkenes (α olefins). Three types of Ziegler–Natta catalysts are currently employed: Solid and supported catalysts based on titanium compounds. They are used in… … Wikipedia
Ziegler-Natta catalyst — ▪ chemistry any of an important class of mixtures of chemical compounds remarkable for their ability to effect the polymerization of olefins (olefin) (hydrocarbons containing a double carbon–carbon bond) to polymers of high molecular… … Universalium
Ziegler — is a common German surname meaning bricklayer , and may refer to the following people:*Adolf Ziegler (1892 1959), German painter, favoured by Adolf Hitler *Alexander Ziegler (1944 1987), a Swiss author and actor *Arthur Ziegler the first… … Wikipedia
Natta, Giulio — ▪ Italian chemist born Feb. 26, 1903, Imperia, near Genoa, Italy died May 2, 1979, Bergamo Italian chemist who contributed to the development of high polymers useful in the manufacture of films, plastics, fibres, and synthetic rubber. Along … Universalium
Karl Ziegler — Infobox Scientist name = Karl Waldemar Ziegler image width = caption = Karl Ziegler birth date = November 26, 1898 birth place = Helsa near Kassel, Germany nationality = Germany death date = death date and age|1973|8|12|1898|11|26 death place =… … Wikipedia
Giulio Natta — Infobox Scientist name = Giulio Natta image width = caption = Giulio Natta birth date = February 26 1903 birth place = Imperia, Italy nationality = Italy death date = death date and age|1979|5|2|1903|2|26 death place = Bergamo, Italy field =… … Wikipedia
Kaminsky catalyst — A Kaminsky catalyst is a catalytic system for alkene polymerization discovered in 1980. Kaminsky catalysts are based on metallocenes of group 4 transition metals with methylaluminoxane (MAO). These catalysts are a type of Ziegler Natta catalyst,… … Wikipedia
Post-metallocene catalyst — A post metallocene catalyst is a kind of catalyst for olefin polymerization. Post metallocene refers to the generation of catalysts following Kaminsky catalysts, which are metallocene catalysts discovered in 1980 by Walter Kaminsky, and have been … Wikipedia
industrial polymers, major — Introduction chemical compounds used in the manufacture of synthetic industrial materials. In the commercial production of plastics, elastomers, man made fibres, adhesives, and surface coatings, a tremendous variety of polymers are… … Universalium
industrial polymers, chemistry of — Introduction structure and composition of chemical compounds made up of long, chainlike molecules (molecule). What distinguishes polymers from other types of compounds is the extremely large size of the molecules. The size of a… … Universalium